**4. Defect stability – formation energy and concentration 34**

**4.1.3. Obtaining the dilute limit with supercell models**

Before considering interacting surface defects, the dilute limit (a single bulk or surface defect
in extended material) is discussed. When the formation energy for an isolated, charged defect
in a periodic model is calculated applying Eq.4.1, the result will depend on the supercell size
and shape. Even for very large supercell sizes, electrostatic interaction between defect and
compensating charge, as well as Coulomb interaction between the defect and its periodic images
will contribute to the computed formation energy. In accordance with a simple electrostatic
model of point charges immersed into the jellium of opposite charge, these interactions scale
as _{ǫL}^{1} , due to Coulomb interaction between defects and compensating charge, for a cubic unit
cell with the supercell lattice constantLcorresponding to the distance between the defect and
its closest images. In the limit of an infinitely large supercell the Coulomb interaction vanishes
and the isolated, non-interacting defect is described. If the dilute limit of an isolated defect

4.1. Stability of an isolated point defect is desired from the calculation of a realistic supercell size (100-1,000 atoms), the effects of Coulomb interaction between defect and compensating charge need to be removed, either by extrapolation or by correction schemes as discussed below, especially in systems with small static dielectric constant.

**Makov-Payne correction scheme**

Various post-processing corrections have been suggested to obtain the dilute limit in super-cell calculations. The most widely used and discussed method for bulk defects is the correc-tion scheme derived by Makov and Payne in 1995 [23] that builds on the work by Leslie and Gillan [143]. They considered an array of point charges compensated by a constant background charge within a structureless dielectric medium with dielectric constant ε. The Makov-Payne correction is

∆E^{corr} = q^{2}α

2εL+2πqQ_{r}

3εL^{3} +O(L^{−5}), (4.20)

whereL = Ω^{3}^{1} is the length of a cubic supercell of volumeΩ,αis the Madelung constant that
depends on the crystal structure (simple cubic, face-centered cubic, or body-centered cubic) and
on the number of basis atoms, andQ_{r}is the second radial moment of the defect charge density

Q_{r}=
Z

Ω

d^{3}rρ_{p}(r)r^{2}. (4.21)

The leading term in Eq.4.20is the screened Madelung lattice energy of point charges [143].

By decomposing the total charge density of a crystal containing a point defect into a periodic
(net neutral) contribution of the underlying crystalρ_{p} and the charge density of the aperiodic
defect, Makov and Payne reproduced this first-order term, and additionally obtained a
third-order correction term representing the interaction between the periodic density and the defect
images.

The Makov-Payne correction scheme has been analyzed in numerous studies [119,122,144–

149]. It has been shown that in most cases it leads to improved convergence to the dilute limit,
*but there are also shortcomings of the method. Lento et al. pointed out that*Qris not necessarily
independent on the supercell size, because the change in the charge density introduced by the
defect need not be well localized as assumed by Makov and Payne [144]. Furthermore, Segev
and Wei found that there may be situations for which the lattice relaxations lead to a symmetry
breaking, and, as a consequence, a net dipole can appear, that would have to be taken into
account [145]. Shim et al. showed that strongly localized charges are far better described by
the Makov-Payne scheme than delocalized ones, by calculating vacancies and interstitials in
diamond [122].

**Freysoldt et al. correction scheme**

*Another correction scheme for bulk defects was suggested in 2009 by Freysoldt et al [150,*151].

The electrostatics in a system containing a charged point defect are analyzed and formulated in terms of the electrostatic potential in this approach.

4.1. Stability of an isolated point defect
The basic idea is to distinguish between two partsE^{inter}andE^{intra}of the correction term to
the charged defect formation energy calculated for a finite cell size.

∆E^{corr}=E^{inter}+E^{intra} (4.22)

E^{inter}is the interaction energy of the defect charge densityq_{d}(r)and the compensating charge
density with the artificial potential due to periodic repetition, andE^{intra}is the interaction energy
of the defect charge density and the background charge density in the reference cell.

To derive the corresponding terms, the creation of charged defects is divided into three steps,
starting from a neutral defect. First, electrons are added to (or removed from) the defect state. An
unscreened defect charge density q_{d}(r) is introduced. Second, electrons are allowed to screen
the introduced charge. This leads to a change in electrostatic potential with respect to the neutral
defectV_{q/0}(r) = V_{defect,q}(r)−V_{defect,0}(r). Third, artificial periodicity and a compensating
homogeneous background charge density n = −_{Ω}^{q} is introduced, leading to a periodic defect
potentialV˜_{q/0}(r). All spurious interactions can be expressed through these quantities, according
to

E^{inter}= 1
2

Z

Ω

d^{3}r[q_{d}(r) +n][ ˜V_{q/0}(r)−V_{q/0}(r)] (4.23)
and

E^{intra}=
Z

Ω

d^{3}r n V_{q/0}(r). (4.24)
The change in potential with respect to the neutral defect is then split into a long-range and a
short-range partV_{q/0}(r) =V_{q}^{lr}(r) +V_{q/0}^{sr} (r). The long-range part

V_{q}^{lr}(r) = 1
ǫ

Z

Ω

d^{3}r^{′} q_{d}(r^{′})

|r−r^{′}| (4.25)

can be calculated analytically using a model charge density forq_{d}(r), for example assuming a
gaussian shape.E^{inter}+E^{intra}is rewritten as a sum of two terms, where the first summand only
contains long-range, and the second only comprises short-range contributions

∆E^{corr} =E_{q}^{lat}−q·∆_{q/0}. (4.26)

The term∆_{q/0} is an alignment term, that suggests potential alignment between systems in
dif-ferent charge states based on the Hartree potential. It can be obtained by calculating V_{q}^{lr}(r)
analytically using Eq.4.25and demanding thatV_{q}^{sr}(r) =V_{q/0}(r)−V_{q}^{lr}(r)must approach zero
far from the defect. Depending on the infrastructure of the applied electronic structure code this
type of level alignment can be convenient.

If the lattice sum
E_{q}^{lat}=

Z

Ω

d^{3}r
1

2[q_{d}(r) +n][ ˜V_{q}^{lr}(r)−V_{q}^{lr}(r)] +nV_{q}^{lr}(r)

(4.27)

4.1. Stability of an isolated point defect
is evaluated using a point charge model distribution, the linear term of the Makov Payne
cor-rection is recovered. In most cases E_{q}^{lat} only weakly depends on the choice of model charge
distribution. This is shown on the example of charged F centers in MgO bulk, for which the
Freysoldt corrections to the formation energies have been calculated using a gaussian charge
distribution for different widths (Table4.1). Up to a gaussian width of 2.0 the Freysoldt
correc-tion yields the same value as the first order Makov-Payne correccorrec-tion to within 0.03 eV.

**Table 4.1.: Freysoldt finite-size correction (in eV) to the formation energies of an F**^{+}and F^{2+}

center in a 64-atom bulk MgO supercell. The corresponding Makov-Payne first-order correc-tions for this example are 0.25 eV and 0.98 eV, respectively. The static dielectric constant of 9.8 and Madelung constant of 2.8373 were used.

Gaussian width F^{+} F^{2+}

0.1 0.25 0.98

0.8 0.25 0.98

2.0 0.25 0.95

**Extrapolation to dilute limit**

Although the correction pre-factors of the Makov-Payne scheme have been questioned, it is
generally accepted that the leading contributions to the bulk defect formation energy dependence
on the supercell size are the terms∼1/Land∼1/L^{3}, whereLis the supercell lattice constant.

This implies that finite-size scaling according to

G^{bulk,q}_{f} (L, ǫ_{F}, µ_{O}) =G^{bulk,q}_{f} (L→ ∞, ǫ_{F}, µ_{O}) +a^{q}_{1}
L + a^{q}_{3}

L^{3} (4.28)

leads to the correct formation energy in the dilute limitG^{bulk,q}_{f} (L→ ∞)[152–154]. Different
variations of this scaling method have been proposed to improve the accuracy of the extrapolated
energy [122,145,155–158].

In Fig.4.2the formation energies for the F^{0}, F^{+}, and F^{2+}center in MgO bulk are shown as a
function of reciprocal supercell length in the oxygen-rich limit for the Fermi level at the VBM.

All cells are fully relaxed, so that all elastic effects are taken into account for the calculated values.

The formation energy of a neutral F center is already converged for a small supercell of 64
atoms, while the formation energies of the F^{+}and the F^{2+}center show a strong dependence on
L, the higher the charge state the more pronounced is the effect. The difference in formation
energy for a 1,728-atom supercell compared to a 1,000-atom supercell is still 50 meV for the
F^{2+} center. Finite size scaling is performed by fitting each set of data (for F^{+} and F^{2+}) to
Eq. 4.28. The extrapolation procedure correctly incorporates the effects of atomic relaxation.

When supercells containing up to 1,728 atoms are calculated for the doubly charged vacancies,

4.1. Stability of an isolated point defect

**Figure 4.2.: Calculated formation energies of bulk F centers (filled symbols) as a function of**
the reciprocal supercell length L^{−1} at PBE level, neglecting vibrations. Formation energies
including the first-order Makov-Payne correction are depicted by open symbols. Solid lines
show finite-size scaling, where supercells of 64 to 1,728 atoms were calculated. Dashed lines
mark the extrapolated formation energies.

using PBE exchange-correlation treatment, the accuracy of the least-square fits is≤0.05eV for the extrapolated values of the formation energies in the dilute limit.

The first-order Makov-Payne correction using the experimental value for the static dielectric constant of MgO (ǫ= 9.8[159]) improves the convergence, but still the computations for large cells are unavoidable to obtain converged results. By comparing the fitting parameters from the extrapolation procedure to the Makov-Payne formula, the static dielectric constant of MgO can be estimated. For DFT-PBE it is 10.70 with electronic and lattice components of 4.88 and 5.82.

The corresponding experimental values are 9.34, 3.01, and 6.33 [160]. The PBE self-interaction error leads to a stronger deviation for the electronic component.

For charged surface defects, modeled using the VCA, the extrapolation is slightly different
due to the broken symmetry at the surface. While for bulk supercells, the formation energies
were fit to Eq.4.28, where a term proportional to _{L}^{1}2 is zero due to symmetry, for the surface
defects this term has to be included. The fitting function used is therefore

G^{VCA,q}_{f} (L,ǫ_{F}, µ_{O}) =G^{VCA,q}_{f} (L→ ∞, ǫ_{F}, µ_{O}) +a^{q}_{1}
L + a^{q}_{2}

L^{2} + a^{q}_{3}

L^{3}. (4.29)
The periodicity of the surface calculations performed in this work is three-dimensional. Slabs
are separated by a vacuum region, and this must be chosen large enough to remove undesired
interactions between repeating slabs. In calculations for differentL, only the lateral dimensions
of the cell are changed, while the vacuum layer thickness is fixed. Since FHI-aims uses

local-4.2. Stability of interacting surface defects in doped material